A hybrid fluoride layered perovskite, (enH<sub>2</sub>)MnF<sub>4</sub>.
Li, Teng; Clulow, Rebecca; Bradford, Alasdair J.; Lee, Stephen L.; Slawin, Alexandra M. Z.; Lightfoot, Philip; Dalton transactions (Cambridge, England : 2003) 48 (2019) 4784–4787; doi:10.1039/c9dt00757a

data_7049150
_publ_section_title
;
 A hybrid fluoride layered perovskite, (enH<sub>2</sub>)MnF<sub>4</sub>.
;
_journal_issue                   15
_journal_name_full
'Dalton transactions (Cambridge, England : 2003)'
_journal_page_first              4784
_journal_page_last               4787
_journal_paper_doi               10.1039/c9dt00757a
_journal_volume                  48
_journal_year                    2019
_chemical_formula_sum            'C2 H10 F4 Mn N2'
_chemical_formula_weight         193.06
_space_group_crystal_system      monoclinic
_space_group_IT_number           14
_space_group_name_Hall           '-P 2ybc'
_space_group_name_H-M_alt        'P 1 21/c 1'
_symmetry_space_group_name_Hall  '-P 2ybc'
_symmetry_space_group_name_H-M   'P 1 21/c 1'
_atom_sites_solution_hydrogens   geom
_audit_creation_method           SHELXL-2016/6
_audit_update_record
;
2018-11-26 deposited with the CCDC.    2019-02-26 downloaded from the CCDC.
;
_cell_angle_alpha                90
_cell_angle_beta                 90.287(6)
_cell_angle_gamma                90
_cell_formula_units_Z            2
_cell_length_a                   8.1735(18)
_cell_length_b                   5.9868(13)
_cell_length_c                   5.9637(14)
_cell_measurement_reflns_used    969
_cell_measurement_temperature    93(2)
_cell_measurement_theta_max      27.4
_cell_measurement_theta_min      2.5
_cell_volume                     291.82(11)
_computing_structure_refinement  'SHELXL-2016/6 (Sheldrick, 2016)'
_computing_structure_solution    'SHELXT 2018/2 (Sheldrick, 2018)'
_diffrn_ambient_temperature      93(2)
_diffrn_detector_area_resol_mean 5.8140
_diffrn_measured_fraction_theta_full 0.996
_diffrn_measured_fraction_theta_max 0.996
_diffrn_measurement_device
;
AFC8: Eulerian 3 circle
;
_diffrn_measurement_device_type
;
Rigaku Pilatus 200K
;
_diffrn_measurement_method       'profile data from \w-scans'
_diffrn_radiation_type           MoK\a
_diffrn_radiation_wavelength     0.71075
_diffrn_reflns_av_R_equivalents  0.0274
_diffrn_reflns_av_unetI/netI     0.0156
_diffrn_reflns_Laue_measured_fraction_full 0.996
_diffrn_reflns_Laue_measured_fraction_max 0.996
_diffrn_reflns_limit_h_max       9
_diffrn_reflns_limit_h_min       -9
_diffrn_reflns_limit_k_max       7
_diffrn_reflns_limit_k_min       -7
_diffrn_reflns_limit_l_max       7
_diffrn_reflns_limit_l_min       -7
_diffrn_reflns_number            3454
_diffrn_reflns_point_group_measured_fraction_full 0.996
_diffrn_reflns_point_group_measured_fraction_max 0.996
_diffrn_reflns_theta_full        25.242
_diffrn_reflns_theta_max         25.265
_diffrn_reflns_theta_min         2.492
_diffrn_source                   'Rotating Anode'
_exptl_absorpt_coefficient_mu    2.258
_exptl_absorpt_correction_T_max  1.000
_exptl_absorpt_correction_T_min  0.632
_exptl_absorpt_correction_type   multi-scan
_exptl_absorpt_process_details   SADABS-2008/1-G.M.Sheldrick
_exptl_crystal_colour            Colorless
_exptl_crystal_density_diffrn    2.197
_exptl_crystal_description       Prism
_exptl_crystal_F_000             194
_exptl_crystal_size_max          0.21
_exptl_crystal_size_mid          0.12
_exptl_crystal_size_min          0.03
_refine_diff_density_max         0.347
_refine_diff_density_min         -0.250
_refine_diff_density_rms         0.066
_refine_ls_extinction_coef       0.075(6)
_refine_ls_extinction_expression Fc^*^=kFc[1+0.001xFc^2^\l^3^/sin(2\q)]^-1/4^
_refine_ls_extinction_method     'SHELXL-2016/6 (Sheldrick 2016)'
_refine_ls_goodness_of_fit_ref   1.123
_refine_ls_hydrogen_treatment    constr
_refine_ls_matrix_type           full
_refine_ls_number_parameters     44
_refine_ls_number_reflns         526
_refine_ls_number_restraints     0
_refine_ls_restrained_S_all      1.123
_refine_ls_R_factor_all          0.0142
_refine_ls_R_factor_gt           0.0141
_refine_ls_shift/su_max          0.000
_refine_ls_shift/su_mean         0.000
_refine_ls_structure_factor_coef Fsqd
_refine_ls_weighting_details
'w=1/[\s^2^(Fo^2^)+(0.0268P)^2^+0.0251P] where P=(Fo^2^+2Fc^2^)/3'
_refine_ls_weighting_scheme      calc
_refine_ls_wR_factor_gt          0.0409
_refine_ls_wR_factor_ref         0.0410
_reflns_Friedel_coverage         0.000
_reflns_number_gt                517
_reflns_number_total             526
_reflns_threshold_expression     'I > 2\s(I)'
_cod_data_source_file            c9dt00757a2.cif
_cod_data_source_block           shelx
_cod_depositor_comments
;
The following automatic conversions were performed:

'_exptl_absorpt_correction_type' value 'Multi-scan' changed to
'multi-scan' according to
/home/data/users/saulius/crontab/automatic-downloads/rss-feeds/RSC/lib/dictionaries/cif_core.dic
dictionary named 'cif_core.dic' version 2.4.2 from 2011-04-26.

Automatic conversion script
Id: cif_fix_values 4973 2017-02-22 13:04:09Z antanas 

 Adding full bibliography for 7049150--7049152.cif.
;
_cod_database_code               7049150
_shelx_shelxl_version_number     2016/6
_shelx_res_checksum              27407